High-strength carbon and low-alloy steels have yield strengths greater
than 275 MPa and can be more or less divided into four classes:
These four types of steels have higher yield strengths than mild carbon
steel in the as-hot-rolled condition. The heat-treated low-alloy steels
and the as-rolled HSLA steels also provide lower ductile-to-brittle
transition temperatures than do carbon steels.
- As-rolled carbon-manganese steels
- As-rolled high-strength low-alloy (HSLA) steels (which are also
known as micro alloyed steels)
- Heat-treated (normalized or quenched and tempered) carbon steels
- Heat-treated low-alloy steels.
These four types of high-strength steels have some basic differences
in mechanical properties and available product forms. In terms of
mechanical properties, the heat-treated (quenched and tempered)
low-alloy steels offer the best combination of strength and toughness.
Structural Carbon Steels
Structural carbon steels include mild steels, hot-rolled carbon-manganese
steels, and heat-treated carbon steels. Mild steels and carbon-manganese
steels are available in all the standard wrought forms: sheet, strip,
plate, structural shapes, bar, bar-size shapes, and special sections.
The heat-treated grades are available as plate, bar and. occasionally,
sheet and structural shapes.
Mild (low-carbon) steels are normally considered to have carbon contents
up to 0.25% C with about 0.4 to 0.7% Mn, 0.1 to 0.5% Si and some residuals
of sulfur, phosphorus, and other elements. These steels are not deliberately
strengthened by alloying elements other than carbon; they contain
some manganese for sulfur stabilization and silicon for deoxidation.
Mild steels are mostly used in the as-rolled, forged, or annealed condition
and are seldom quenched and tempered.
The largest category of mild steels is the low-carbon
(<0.08% C, with <0.4% Mn) mild steels used for forming and packaging.
Mild steels with higher carbon and manganese contents have also been used
for structural products such as plate, sheet, bar, and structural sections.
High-strength structural carbon steels have yield strengths greater than
275 MPa and are available in various product forms:
The heat treatment of carbon steels, which typically attain yield
strengths of 290 to 690 MPa, consists of either normalizing or quenching
and tempering. These heat treatments can be used to improve the mechanical
properties of structural plate, bar, and occasionally, structural shapes.
- Cold-rolled structural sheet
- Hot-rolled carbon-manganese steels in the form of sheet, plate, bar, and structural shapes
- Heat-treated (normalized or quenched and tempered) carbon steels in the form of
plate, bar, and occasionally, sheet and structural shapes.
Normalizing involves air-cooling from austenitizing temperatures and
produces essentially the same ferrite-pearlite microstructure as that
of hot-rolled carbon steel, except that the heat treatment produces a
finer grain size. This grain refinement makes the steel stronger, tougher,
and more uniform throughout.
Quenching and tempering, that is heating to about 900oC, water
quenching, and tempering at temperatures of 480 to 600oC or
higher, can provide a tempered martensitic or bainitic microstructure that
results in better combinations of strength and toughness. An increase in
the carbon content to about 0.5%, usually accompanied by an increase in
manganese, allows the steels to be used in the quenched and tempered
Quenched and Tempered Low-Alloy Steel
Alloy steels are defined as those steels that:
The low-alloy steels are those steels containing alloy elements,
including carbon, up to a total alloy content of about 8.0%.
- contain manganese, silicon, or copper in quantities greater than the
maximum limits (1.65% Mn, 0.60% Si, and 0.60% Cu) of carbon steel; or
- that have specified ranges or minimums for one or more other alloying
Except for plain carbon steels that are micro alloyed with just vanadium,
niobium, and/or titanium, most low-alloy steels are suitable as engineering
quenched and tempered steels and are generally heat treated for engineering
use. Low-alloy steels with suitable alloy compositions have greater
hardenability than structural carbon steel and, thus, can provide high
strength and good toughness in thicker sections by heat treatment.
Their alloy contents may also provide improved heat and corrosion
resistance. However, as the alloy contents increase, alloy steels
become more expensive and more difficult to weld. Quenched and
tempered structural steels are primarily available in the form of
plate or bar products.
Alloying Elements and Their Effect on Hardenability and Tempering.
Quenched and tempered steels have carbon contents in the range of 0.10 to
0.45%, with alloy contents, either singly or in combination, of up to 1.5%
Mn, 5% Ni, 3% Cr, 1% Mo, 0.5% V, 0.10% Nb; in some cases they contain small
additions of titanium, zirconium and/or boron. Generally, the higher the
alloy content, the greater the hardenability and the higher the carbon
content, the greater the available strength. The response to heat
treatment is the most important function of the alloying elements
in these steels.
Microalloyed Quenched and Tempered Grades. Although fittings with 0.69% Mn
and induction bends use quenching and tempering as a standard practice,
mild steels (plain, low-carbon steels with less than 0.7% Mn) with
microalloying additions of vanadium, niobium, or titanium are seldom
used as quenched and tempered steels.
However, elements such as boron and vanadium are considered as substitutes
for other elements that enhance hardenability. The titanium was added in
order to form titanium nitride, thereby retaining an increased amount of
vanadium in solution. This provided for a more efficient use of vanadium
as a hardenability agent.
Some scientist investigated completely V-substituted variants of
4140 base series (0.4C-1Cr) with titanium additions, as well as partially
V-substituted variants with and without titanium additions. These studies
The pronounced effect on hardenability of molybdenum-vanadium combinations
without titanium as observed by Manganon in 4330 steels, can probably be
reconciled with the third result of Sandberg in that the latter studied
steels containing 0.06% Al, which would be expected to remove nitrogen
to about the same extent as 0.04% Ti.
- Complete substitution of molybdenum by vanadium does not increase the
hardenability over standard 4140 (0.20% Mo) even when all the vanadium is
dissolved during austenitization
- Steels containing 0.1 to 0.2% V and 0.04% Ti are characterized by
significantly increased hardenability (10 to 25% in D1) over standard 4140
- Microalloy combinations of V + Mo + Ti (~0.06-0.06-0.04%) provide
very high hardenability with D1 being up to 60% greater than the D1, in
standard 4140 with 0.20% Mo. This effect is completely absent in partially
substituted steel without titanium.
Quenched and tempered alloy steels can offer a combination of high strength
and good toughness. In addition, quenched and tempered alloy steel plate
is available with ultrahigh strengths and enhanced toughness. Enhanced
toughness and high strength are achieved in the nickel-chromium-molybdenum
alloys, which include steels such as ASTM A 543, HY-80, HY-100 and HY-130.
These steels use nickel to improve toughness.
High-Nickel Steels for Low-Temperature Service. For applications involving
exposure to temperatures from 0 to -195oC, the ferritic steels with high
nickel contents are typically used. Such applications include storage
tanks for liquefied hydrocarbon gases and structures and machinery
designed for use in cold regions. These steels utilize the effect of
nickel content in reducing the impact transition temperature, thereby
improving toughness at low temperatures. Carbon and alloy steel castings
for subzero-temperature service are covered by ASTM standard
specification A 757.
The 5% Ni alloys for low-temperature service include HY-130 and ASTM A 645.
For steel purchased according to ASTM A 645 minimum Charpy V-notch impact
requirements for 25 mm plate are designated at -170oC for hardened,
tempered, and reversion-annealed plate.
Double normalized and tempered 9% nickel steel is covered by ASTM A 353,
and quenched and tempered 8% and 9% nickel steels are covered by ASTM A 553
(types I and II). For quenched and tempered material, the minimum lateral
expansion in Charpy V-notch impact tests is 0.38 mm. Testing of typical
tensile properties of 5% and 9% Ni steels at room temperature and at
subzero temperatures shows that yield and tensile strengths increase
as testing temperature is decreased. These steels remain ductile at
the lowest resting temperatures.
Ferritic nickel steels are too tough at room temperature for valid fracture
toughness (KIc) data to be obtained on specimens of reasonable
size, but limited fracture toughness data have been obtained on these
steels at subzero temperatures by the J-integral method. The 5% Ni steel
retains relatively high fracture toughness at -162oC and the 9% Ni steel
retains relatively high fracture toughness at -196oC. These temperatures
approximate the minimum temperatures at which these steels may be used.